The interaction between the spin transition and a crystallographic phase transition in the spin-crossover compound [Fe(bbtr) 3 ](ClO 4 ) 2 : Nucleation, formation of domains and ﬂuctuations Itana Krivokapic a , Cristian Enachescu b, * , Robert Bronisz c , Andreas Hauser a, * a Département de chimie physique, Université de Genève, 30, quai Ernest-Ansermet, 1211 Genève 4, Switzerland b Department of Physics, Al. I. Cuza University, 700506 Iasi, Romania c Faculty of Chemistry, University of Wroclaw, F. Joliot-Curie 14, 50-383 Wroclaw, Poland article info Article history: Received 28 February 2008 Received in revised form 6 March 2008 Accepted 10 March 2008 Available online 19 March 2008 Dedicated to Dante Gatteschi in honour of his contribution in the ﬁeld of molecular magnetism. Keywords: Iron(II) spin-crossover complex High-spin ? low-spin relaxation Crystallographic phase transition Light-induced spin transition abstract The thermal and the light-induced spin transition in [Fe(bbtr) 3 ](ClO 4 ) 2 (bbtr = 1,4-di(1,2,3-triazol-1-yl)) as well as the high-spin ? low-spin relaxation following the light-induced population of the high-spin state below the thermal transition temperature are discussed in relation to the accompanying crystallo- graphic phase transition. The experimental data have exclusively been obtained using optical single crys- tal absorption spectroscopy. Ó 2008 Elsevier B.V. All rights reserved. 1. Introduction Spin-crossover compounds  are compounds of octahedral complexes of transition metal ions having d 4 to d 7 electron conﬁg- urations. They are among the few systems showing bistability at a molecular scale with switchable properties induced by variations of temperature [2,3], pressure [4,5] or by light-irradiation . This makes them interesting for potential application such as high-den- sity information storage systems  and displays . By far the largest number of known spin-crossover systems have d 6 iron(II) as central ion, for which the transition occurs between the low- spin (LS) 1 A 1 ðt 6 2g Þ state and the high-spin (HS) 5 T 2 ðt 4 2g e 2 g Þ state. The thermal transition is entropy driven by both the electronic degeneracy of the HS state as well as the vibrational contribution, and it always occurs from the diamagnetic LS state populated at low temperatures to the paramagnetic HS state populated at ele- vated temperatures. Due to elastic interactions between the spin- crossover units resulting from the large difference in metal–ligand lengths between the two spin states, the thermal spin transition is very often much more abrupt than predicted by a simple Boltz- mann distribution between the two vibronic manifolds. If the elas- tic interactions between the spin-crossover units are large enough, it may even occur as a ﬁrst order transition and show a thermal hysteresis [2,3]. Such cooperative effects have been and continue to be of interest, as they constitute an essential ingredient for the macroscopic bistability and memory effects needed for the above-mentioned potential applications. Of particular interest, in the context of the work presented in this paper, are systems in which the spin transition triggers a crystallographic phase transi- tions as for instance in the model compound [Fe(ptz) 6 ](BF 4 ) 2 (ptz = 1-propyltetrazole) [9–12], or induces a super-structure such as in [Fe(pic) 3 ]Cl 2 EtOH [13,14], and may even lead to a self-grind- ing effect reducing the crystallite size to a comparatively homoge- neous distribution of the order of micrometres . At low temperatures iron(II) spin-crossover systems can be switched from the ground LS state to the long lifetime metastable HS state by using light of appropriate wavelengths, a phenomenon known as Light-Induced Excited Spin State Trapping (LIESST) [2,16]. The at low temperatures metastable HS state relaxes towards the ground state by a non-adiabatic, non-radiative process , that is by a slow tunnelling process below 50 K and thermal activation above that temperature. Cooperative effects also inﬂuence the kinet- 0020-1693/$ - see front matter Ó 2008 Elsevier B.V. All rights reserved. doi:10.1016/j.ica.2008.03.064 * Corresponding authors. E-mail addresses: [email protected](C. Enachescu), andreas.hau- [email protected](A. Hauser). Inorganica Chimica Acta 361 (2008) 3616–3622 Contents lists available at ScienceDirect Inorganica Chimica Acta journal homepage: www.elsevier.com/locate/ica
Inorganica Chimica Acta 361 (2008) 3616–3622
Contents lists available at ScienceDirect
Inorganica Chimica Acta
journal homepage: www.elsevier .com/locate / ica
The interaction between the spin transition and a crystallographic phasetransition in the spin-crossover compound [Fe(bbtr)3](ClO4)2: Nucleation,formation of domains and fluctuations
Itana Krivokapic a, Cristian Enachescu b,*, Robert Bronisz c, Andreas Hauser a,*
a Département de chimie physique, Université de Genève, 30, quai Ernest-Ansermet, 1211 Genève 4, Switzerlandb Department of Physics, Al. I. Cuza University, 700506 Iasi, Romaniac Faculty of Chemistry, University of Wroclaw, F. Joliot-Curie 14, 50-383 Wroclaw, Poland
a r t i c l e i n f o a b s t r a c t
Article history:Received 28 February 2008Received in revised form 6 March 2008Accepted 10 March 2008Available online 19 March 2008
Dedicated to Dante Gatteschi in honour ofhis contribution in the field of molecularmagnetism.
The thermal and the light-induced spin transition in [Fe(bbtr)3](ClO4)2 (bbtr = 1,4-di(1,2,3-triazol-1-yl))as well as the high-spin ? low-spin relaxation following the light-induced population of the high-spinstate below the thermal transition temperature are discussed in relation to the accompanying crystallo-graphic phase transition. The experimental data have exclusively been obtained using optical single crys-tal absorption spectroscopy.
� 2008 Elsevier B.V. All rights reserved.
Spin-crossover compounds  are compounds of octahedralcomplexes of transition metal ions having d4 to d7 electron config-urations. They are among the few systems showing bistability at amolecular scale with switchable properties induced by variationsof temperature [2,3], pressure [4,5] or by light-irradiation . Thismakes them interesting for potential application such as high-den-sity information storage systems  and displays . By far thelargest number of known spin-crossover systems have d6 iron(II)as central ion, for which the transition occurs between the low-spin (LS) 1A1ðt6
2gÞ state and the high-spin (HS) 5T2ðt42ge2
gÞ state.The thermal transition is entropy driven by both the electronicdegeneracy of the HS state as well as the vibrational contribution,and it always occurs from the diamagnetic LS state populated atlow temperatures to the paramagnetic HS state populated at ele-vated temperatures. Due to elastic interactions between the spin-crossover units resulting from the large difference in metal–ligandlengths between the two spin states, the thermal spin transition is
ll rights reserved.
. Enachescu), andreas.hau-
very often much more abrupt than predicted by a simple Boltz-mann distribution between the two vibronic manifolds. If the elas-tic interactions between the spin-crossover units are large enough,it may even occur as a first order transition and show a thermalhysteresis [2,3]. Such cooperative effects have been and continueto be of interest, as they constitute an essential ingredient for themacroscopic bistability and memory effects needed for theabove-mentioned potential applications. Of particular interest, inthe context of the work presented in this paper, are systems inwhich the spin transition triggers a crystallographic phase transi-tions as for instance in the model compound [Fe(ptz)6](BF4)2
(ptz = 1-propyltetrazole) [9–12], or induces a super-structure suchas in [Fe(pic)3]Cl2 � EtOH [13,14], and may even lead to a self-grind-ing effect reducing the crystallite size to a comparatively homoge-neous distribution of the order of micrometres .
At low temperatures iron(II) spin-crossover systems can beswitched from the ground LS state to the long lifetime metastableHS state by using light of appropriate wavelengths, a phenomenonknown as Light-Induced Excited Spin State Trapping (LIESST)[2,16]. The at low temperatures metastable HS state relaxes towardsthe ground state by a non-adiabatic, non-radiative process , thatis by a slow tunnelling process below�50 K and thermal activationabove that temperature. Cooperative effects also influence the kinet-
I. Krivokapic et al. / Inorganica Chimica Acta 361 (2008) 3616–3622 3617
ics of the relaxation process, resulting in highly non-exponentialrelaxation curves . In some compounds, a reverse photophysicalprocess with irradiation at 830 nm known as reverse-LIESST can alsoreconvert the light-induced HS state back to the ground state .
The most simple model treats the cooperative effects in a mean-field approach [19,20]. This model was successfully applied to anumber of systems with moderate interaction parameters[18,21,22], but its performance was less satisfactory for stronglycooperative systems showing hysteresis behaviour. Some 18 yearsago, Sorai et al.  suggested that in such systems the spin tran-sition occurs through domains of like spins, that is, through the for-mation of domains consisting of molecules of the same spin state.Over the past few years, the existence of such like spin domainswas inferred from experimental data, namely the observation ofminor hysteresis loops for thermal and light-induced thermal tran-sitions [24,25], X-ray diffraction data , Raman scattering duringthe thermal transition , and neutron Laue scattering on singlecrystals . Several models derived mainly from the analysis ofdomains in magnetic systems such as Preisach type models or the First Order Reversal Curves (FORC) method [29–31] revealedthat in the case of powder samples the domains may be regardedas independent.
In the present paper we discuss the formation and existence oflike spin domains in single crystals of [Fe(bbtr)3](ClO4)2
(bbtr = 1,4-di(1,2,3-triazol-1-yl)) during the thermal spin transitionas well as during relaxation following irradiation. This compoundpresents a 2D polymeric type structure with every Fe2+ centre sur-rounded by six ligands and every ligand acting as bridging ligand be-tween two Fe2+ centres. This results in a high degree of cooperativity,which manifests itself in a thermal spin transition with a 15 K widehysteresis centred around 105 K. The system presents two crystallo-graphic phases: an ordered phase at above the spin transition tem-perature having space group P�3, and a disordered phase below thespin transition temperature for which to date it has not been possibleto determine the crystal structure . The crystallographic phasetransition from ordered to disordered phase has been associatedwith a nucleation and growth process and domain formation in aprevious communication . In order to clarify the complex behav-iour of this system, we provide in this paper a full analysis of its ther-mal spin transition, low temperature photoexcitation and finally ofthe relaxation curves inside the thermal hysteresis.
See the paper by Bronisz  for a detailed account of the syn-thesis, crystal growth and high-temperature crystal structuredetermination of the title compound. The high-quality [Fe(bbtr)3](ClO4)2 crystals of �0.4 � 0.4 � 0.2 mm3 used in the present studywere likewise grown by Bronisz. They are hexagonal with well-developed faces, transparent at room temperature and red at cryo-genic temperatures. They cleave easily perpendicular to the c-axis.The experimental data presented in this paper were exclusively ob-tained from optical absorption measurements on single crystals.For these measurements, crystals cleaved to approximately 60 lmthickness were mounted on a small aperture in a copper sampleholder using silver contact glue. For temperature dependant mea-surements between cryogenic and room temperature, the sampleholder was inserted into a closed cycle cryostat capable of achievingtemperatures down to 4 K (Janis Research) and equipped with aprogrammable temperature controller allowing variable tempera-ture scans. For irradiation experiments involving LIESST andreverse-LIESST at temperatures below 20 K, the light of a continu-ous Ar/Kr mixed gas laser at 488 nm (Spectra Physics 2018) or ofa Xe-arc lamp and a laser diode at 830 nm (ILEE Model Z40KV1)were used, respectively. With laser powers of �6 mW/mm2 a
quantitative population of the HS state was achieved in <30 s.High-quality absorption spectra between 9000 and 28000 cm�1
(400–900 nm) were recorded on a Fourier transform spectrometer(Bruker IFS66) equipped with the respective beam splitters anddetectors. Kinetic experiments at fixed temperatures and tempera-ture scan experiments were performed on a home-built systemconsisting of a 0.28 m monochomator (Spex 280M, holographicgrating with 150 grooves/mm) equipped with a CCD camera (Jo-bin-Yvon Spex CCD 3500) and polychromatic light from a 50 Wtungsten halogen lamp as probe beam. This set-up allowed record-ing a full spectrum between 10000 and 25000 cm�1 at given timeintervals, the minimum time interval between two spectra being3 s. In order to minimize the amount of light from the 50 W tung-sten halogen lamp falling on the sample, neutral density filters wereused to attenuate the light to <2% of its full intensity and the probebeam was gated with a shutter in parallel to the shutter of the CCDcamera. Thus the effects of the probe beam are negligible with re-gard to the light-induced spin transition. For the HS ? LS relaxationexperiments at a fixed temperature, the initial population of the HSwas achieved below 20 K using comparatively high laser powers of20 mW/mm2, then the temperature was raised to the target tem-perature within <2 min. The laser was kept on the sample until thistemperature was reached, and switched off as the relaxation exper-iment was started. This procedure ensured that even for relaxationcurves at comparatively high-temperatures, that is, approachingthe thermal transition temperature, the initial HS population wasclose to 100%. For additional irradiation experiments inside thethermal hysteresis, a frequency doubled pulsed Nd:YAG laser(Quantel Brilliant B) was used.
For both the temperature dependent absorption spectra as wellas the time dependent spectra, the fraction of complexes in the HSstate can be extracted from the relative intensities of the typicalabsorption bands of the HS and the LS species . By recordingfull spectra, artefacts due to baseline shifts from variations in dif-fuse scattering can be eliminated. For the analysis of the tempera-ture dependent spectra, the small temperature dependence of theoscillator strength of the respective transition was neglected.
3. Results and discussion
3.1. Absorption spectra during the thermal spin transition
Fig. 1 shows the high-quality single crystal absorption spectraof [Fe(bbtr)3](ClO4)2 with the light propagating along the c-axis(a spectrum) at 295 K and at 10 K on slow cooling. At room tem-perature, when all complexes are in the HS state, the spectrumshows the typical near infrared band of the HS species centred at12000 cm�1 (833 nm) corresponding to the 5T2 ?
5E ligand-fieldtransition. The 10 K spectrum is characteristic for the LS specieswith the more intense absorption band in the visible centred at18000 cm�1 (590 nm) and corresponding to the 1A1 ? 1T1 ligand-field transition. In accordance with magnetic susceptibilitymeasurements on a polycrystalline sample  the thermal spintransition is complete with neither a residual HS fraction at lowtemperature nor a residual LS fraction at high-temperature.
With temperature quenching, that is, very fast cooling at >60 K/min starting from room temperature down to <60 K, the complexescan be trapped almost quantitatively in the HS state. Fig. 1 includesthe absorption spectrum of the title compound at 10 K in thistrapped HS state, with a LS fraction of only �10%. At 10 K the tem-perature quenched HS state has a very long lifetime. This is dis-cussed in more detail in Section 3.4.
Fig. 2 shows the absorption spectrum of the title compound as afunction of decreasing temperature between 110 and 90 K at acooling rate of 0.03 K/min on starting from room temperature.
Fig. 1. Single crystal absorption spectrum of [Fe(bbtr)3](ClO4)2 at 295 K (—) and at10 K on slow cooling (. . .) and after temperature quenching (---).
Fig. 2. Single crystal absorption spectrum of [Fe(bbtr)3](ClO4)2 (d = 60 lm) duringthe thermal transition on cooling with a rate of 0.03 K/min from room temperature(top sheet) and from 120 K on the second cycle (bottom sheet).
Fig. 3. Single crystal absorption spectra of [Fe(bbtr)3](ClO4)2 at 10 K before (. . .) andafter (---) broad band irradiation using a Xenon arc lamp, followed by irradiation at830 nm using a red laser diode (—).
3618 I. Krivokapic et al. / Inorganica Chimica Acta 361 (2008) 3616–3622
While decreasing the temperature, the HS band in the near infrareddisappears abruptly at around 100 K and is replaced by the moreintense LS band in the visible, indicating that the thermal HS ? LStransition occurs at T#c � 100 K. Concomitantly with the spin tran-sition a marked baseline shift in the optical spectrum is observed.This is due to an increase in wavelength independent diffuse scat-tering, and indicates that at the spin transition temperature do-mains with a domain size of the order of the wavelength of lightdevelop. This effect occurs right at the beginning of the transitionwhen the LS fraction is still low, indicative of a nucleation andgrowth process. On heating the crystal to 120 K, that is, abovethe thermal LS ? HS transition at T"c � 113 K , and subsequentcooling down at the same rate, the thermal HS ? LS transition
occurs at distinctly higher temperature than on the first coolingdown. This is to be discussed in some detail in Section 3.3. Thepoint to note here is that the accompanying baseline shift is muchsmaller than on the first cooling cycle. Thus even though at 120 K aHS fraction of 1 is restored, the system keeps a memory of the do-main structure resulting form the first cooling cycle. This domainstructure is only annealed upon heating the sample to above 200 K.
3.2. LIESST, reverse-LIESST and the HS ? LS relaxation at lowtemperature
As mentioned in the introduction, many spin-crossover sys-tems, especially those with triazole and tetrazole ligands exhibitthe phenomenon of LIESST. Fig. 3 shows the absorption spectrumof the title compound at 10 K before and after irradiation with abroad band Xenon arc lamp. Irradiation completely bleaches thecharacteristic LS absorption bands indicating a quantitativeLS ? HS transformation. At 10 K the system remains trapped inthis metastable HS state for a very long time because of the largeenergy barrier between the two states resulting from the largebond length difference and at the same time small energy differ-ence. At temperatures >50 K, relaxation back to the LS ground statesets in (see below). The system can also be reconverted to the LSstate at 10 K by irradiating at 830 nm, that is, into the near-infraredband of the HS species. Fig. 3 includes the corresponding absorp-tion spectrum after prolonged irradiation at 830 nm (2 mW/mm2) showing that in reverse-LIESST a saturation value of the LSfraction of 85% is obtained .
Quantitative photoexcitation experiments were performed at10 K using the 488 nm line of an Ar–Kr cw laser. Fig. 4 shows pho-toexcitation curves obtained from recording full absorption spectraat given time intervals for three different light intensities. The timenecessary to populate the HS state quantitatively is 30 s for a laserpower of �6 mW/mm2 at the sample. With a laser power of0.02 mW/mm2 a quantitative population of the HS state can stillbe achieved, but it takes more than 1 h to do so. As describedabove, the contribution to the photoexcitation from the W-halogen
Fig. 4. Photoexcitation curves for the LS ? HS transformation of [Fe(bbtr)3](ClO4)2
at 10 K during irradiation with different intensities of the 488 nm line of an Ar–Krcw laser.
I. Krivokapic et al. / Inorganica Chimica Acta 361 (2008) 3616–3622 3619
lamp is negligible. At 488 nm the optical density of the thin crystalused was <0.2 mm, thus no significant concentration gradientswere introduced by the irradiation. No significant incubation timewas observed, indeed, the photoexcitation curves are close to sin-gle exponential and indicate a quantum efficiency of close to unity,in line with previously reported values [6,35].
Below 50 K the relaxation of the light-induced HS state is tooslow to be measured; only above this temperature can it be fol-lowed within a reasonable time. Fig. 5 shows absorption spectraduring the HS ? LS relaxation recorded at 52 K following the quan-titative light-induced population of the HS state. In comparison tothe thermal spin transition, the baseline shift accompanying the
Fig. 5. Single crystal absorption spectra during HS ? LS relaxation of [Fe(bbtr)3](ClO4)2 following LIESST at 52 K.
relaxation after photoexcitation is much smaller, indicating thatduring the relaxation no additional crystal defects are created.
Fig. 6 shows HS ? LS relaxation curves plotted as the HS frac-tion, cHS, versus time at different temperatures following the quan-titative population of the HS state at 10 K and quickly warming tothe target temperature. As observed for a number of related com-pounds, the relaxation curves are sigmoidal, confirming the coop-erative character of the spin transition in the compound underinvestigation. The total relaxation time is more then 7 h at 50 K,it decreases with increasing temperature to 4 h at 55 K and toabout 5 min at 65 K. The relaxation curves are reasonably well de-scribed by the mean-field equation for cooperative effects, whichrelates the relaxation rate constant, kHL, to the LS fraction in anauto-accelerating fashion 
kHLðT; cLSÞ ¼ ðT; cLS ¼ 0Þ � eaðTÞcLS ð1Þ
Fig. 6. HS ? LS relaxation curves of [Fe(bbtr)3](ClO4)2 following LIESST at varioustemperatures, derived from optical spectra as shown in Fig. 5 for T = 52 K.
3620 I. Krivokapic et al. / Inorganica Chimica Acta 361 (2008) 3616–3622
with a the acceleration factor. Based on the mean-field model kHL
(T, cLS = 0) should follow an Arrhenius like behaviour above 50 Kand a should decrease as 1/T. However, best fits using Eq. (1) doshow systematic deviations from the experimental curves, theacceleration factor a � 6.5 is almost temperature independent overthe whole temperature range, and at temperatures above 70 K therelaxation even though initially still becoming faster with increas-ing temperature is slower than expected. Finally the HS ? LS relax-ation even slows down as the thermal transition temperature of100 K is approached. This can only be explained by quite largeshort-range interactions leading to fluctuations and the formationof clusters or domains of equal spins [33,36,37].
3.3. The thermal hysteresis
Fig. 7a shows a series of thermal hysteresis loops measured fol-lowing different protocols. Basically they all are in agreement with
Fig. 7. (a) The thermal spin transition of a single crystal of [Fe(bbtr)3](ClO4)2 fordifferent temperature sweep rates and thermal histories of the crystal. (b) Thethermal hysteresis of different single crystals of [Fe(bbtr)3](ClO4)2 for a temperaturesweep rate of 0.1 K/min and different thermal histories, as well as after irradiation.
the published curve as determined from magnetic susceptibilitymeasurements on a polycrystalline powder  showing a hyster-esis of approximately 15 K. However, for the single crystals theyare much steeper, as previously observed for other spin transitioncompounds . More importantly, the hysteresis width depends(i) on the temperature sweep rate, indicating that the kinetics ofthe associated phase transition are very slow indeed, and (ii) onthe history of the crystal: when starting from room temperaturethe apparent transition temperature for the HS ? LS transition islower than when coming from below the thermal transition, heat-ing up to 120 K and then decreasing the temperature again. Thus,at a sweep rate of 0.1 K/min, T#c � 97 K when coming from roomtemperature and 102 K when coming from 120 K following thefirst cycle.
Fig. 7b shows the hysteresis loops for two different crystals.Whereas T#c differs by 6 K when cooling down from the high-tem-perature phase, it takes on the same value of 102 K for both crys-tals for the second cycle starting from 120 K. Irrespective of thehistory of the crystals the LS ? HS transition temperature on heat-ing, T"c, remains the same at 113 K.
In line with this observation goes the fact that the crystallo-graphic structure could be obtained for the HS state at 135 K, butfor the LS state at 80 K it failed . All this leads to the conclusionthat the thermal spin transition triggers a crystallographic phasetransition and that below T#c the low-temperature phase has a highdegree of disorder. On the first cooling cycle this crystallographicphase transition occurs as a nucleation and growth process and re-sults in the formation of a domain structure  depending uponthe individual crystal. Upon heating to 120 K, the system returnsto the HS state, but retains some memory of this domain structure.
Despite the small temperature sweep rates of the experiment,the apparent transition temperature on cooling depends uponthe sweep rate. This indicates that the relaxation is very slowand is governed by the macroscopic nuclear rearrangements ofthe crystallographic phase transition rather by the intersystemcrossing process of the HS ? LS relaxation. As shown in Fig. 8,the two different cooling protocols result in very different relaxa-tion curves, measured at constant temperatures just below therespective transition temperatures. As expected for a nucleationand growth process, on cooling from room temperature, the relax-ation curves show an initial very slow decrease in the HS fractionfor the nucleation process, followed by the typical acceleration ofa growth process. For the second cycle, the relaxation curves are al-most single exponential. Thus on the second cooling cycle, the pre-formed domains relax to the LS state in a stochastic process.
Interestingly, the HS ? LS relaxation curves also depend uponcrystal quality and size. The curves in Fig. 8a were recorded on acomparatively large crystal (diameter �0.5 mm) with a non-negli-gible number of easily discernible defects under a microscope.Fig. 8b shows relaxation curves on cooling from 120 K to the targettemperature for a small high-quality crystal (diameter �0.3 mm).The relaxation curves are clearly different from the ones inFig. 8a. The curves at 101 K are quite similar, the relaxation beingcomplete after �250 s. At somewhat higher temperature, therelaxation curves for the high-quality crystal instead of being com-paratively smooth, show distinct steps. This indicates that in thehigh-quality crystal the number of domains formed during therelaxation process is smaller. The fact that the steps for the curvesrecorded at different temperatures have roughly the same height isin line with the above mentioned memory effect.
3.4. The temperature quenched state
A key question regards the nature of the temperature quenchedHS state: is it similar to the light-induced HS state or are there sig-nificant differences. As mentioned above, it has so far not been pos-
Fig. 8. (a) Relaxation curves for a [Fe(bbtr)3](ClO4)2 single crystal at different te-mperatures when starting the experiment from room temperature (open symbols),and from 120 K on the second cycle (full symbols), adapted from Ref. .(b) HS ? LS relaxation curves for a small high-quality crystal around T#c. (c) H-S ? LS relaxation curves at 60 and 65 K, after temperature quenching (open sym-bols) and following irradiation (full symbols).
I. Krivokapic et al. / Inorganica Chimica Acta 361 (2008) 3616–3622 3621
sible to determine crystal structures below 110 K. A tentative an-swer can be obtained from the comparison of HS ? LS relaxation
curves obtained after thermal quenching on the one hand and afterirradiation on the other hand. Fig. 8c shows corresponding relaxa-tion curves at 60 and 65 K. The experimental curves at the twotemperatures obtained by the two different procedures are identi-cal within experimental error. This indicates that the two metasta-ble HS states are structurally very similar. Provided that thetemperature-quenched structure is not too different from the roomtemperature structure this, in turn, means that the low-tempera-ture irradiation reinstalls some order into the system. This can becorrelated to the observation reported in reference , that therelaxation curves obtained after irradiation in the neighbourhoodof the thermal hysteresis are more in line with the curves of thesample cooled directly from the fully ordered room temperaturephase rather than the ones obtained after a thermal hysteresiscycle. This is further supported by the following experiment: acrystal is first quenched from room temperature to 20 K, thusfreezing in a HS fraction of 90%. The 10% LS fraction is convertedto HS by irradiation and the crystal is warmed to 120 K under con-stant irradiation such that at all times it is in the HS state. Asshown in Fig. 7b, on subsequent slow cooling, the thermal transi-tion curve is identical to the one observed for the cooling cyclestarting from room temperature.
The two-dimensional polymeric spin-crossover compound[Fe(bbtr)3](ClO4)2 shows some remarkable features in its thermalbehaviour. The direct bridging of the iron(II) centres in a triangulararrangement results in comparatively strong elastic interactionsand hysteresis behaviour. At room temperature, that is, in the HSstate, the crystal shows an ordered structure. The spin transition it-self triggers a crystallographic phase transition such that at lowtemperatures, that is, in the LS state, the structure shows a strongdegree of disorder. On the first cooling cycle the crystallographicphase transition occurs as a nucleation and growth process andresults in the formation of a domain structure with a domain sizeof the order of the wavelength of light. On subsequent heating tojust above T"c and renewed cooling the shows a memory effect ofthe domain structure. The HS ? LS relaxation curves followingthe light-induced population of the HS state at low temperaturesshow the sigmoidal shape typical for spin-crossover systems withstrong cooperative effects. The thermal transition temperaturebeing comparatively low, it is possible to maintain the system inthe light-induced HS state all the way up to the transition temper-ature. Near the transition temperature, the HS ? LS relaxationslows down. This is contrary to mean-field theory of cooperativeeffects and can only be explained by considering strong nearestneighbour interactions leading to fluctuations, and nucleationand growth phenomena. It should be possible to follow the domainformation by temperature dependant optical microscopy. Likewise,pulsed irradiation inside the thermal hysteresis as first demon-strated by Freysz et al. , could give further insight.
We thank the MAGMANet Network of Excellence of the Euro-pean Union (Contract: NMP3-CT-2005-515767-2) and the SwissNational Science Foundation for financial support. CE thanks toPNCDI II Romanian CNCSIS Grant ‘‘IDEI”.
 P. Gütlich, H.A. Goodwin (Eds.), Spin Crossover in Transition Metal CompoundsI–III, Top. Curr. Chem., vol. 233–235, Springer, Heidelberg, 2004.
 P. Gütlich, A. Hauser, H. Spiering, Angew. Chem. 106 (1994) 2971. P. Gütlich, A. Hauser, H. Spiering, Angew. Chem., Int. Ed. 33 (1994) 2024. P. Gütlich, A.B. Gaspar, Y. Garcia, Y.V. Ksenofontov, C. R. Chim. 10 (2007) 21.
3622 I. Krivokapic et al. / Inorganica Chimica Acta 361 (2008) 3616–3622
 P. Gütlich, V. Ksenofontov, A.B. Gaspar, Coordin. Chem. Rev. 249 (2005)1811.
 A. Hauser, Top. Curr. Chem. 234 (2004) 155. J.F. Letard, P. Guionneau, L. Goux-Capes, Top. Curr. Chem. 235 (2004) 221. J.P. Gaudry, L. Capes, P. Langot, S. Marcen, M. Kollmannsberger, O. Lavastre, E.
Freysz, J.F. Letard, O. Kahn, Chem. Phys. Lett. 324 (2000) 32. J. Jeftic, H. Romstedt, A. Hauser, J. Phys. Chem. Solids 57 (1996) 1743.
 J. Jeftic, A. Hauser, J. Phys. Chem. B 101 (1997) 10262. N.O. Moussa, G. Molnar, X. Ducros, A. Zwick, T. Tayagaki, K. Tanaka, A.
Bousseksou, Chem. Phys. Lett. 402 (2005) 503. L.H. Böttger, A.I. Chumakov, C.M. Grunert, P. Gütlich, J. Kusz, H. Paulsen, U.
Ponkratz, V. Rusanov, A.X. Trautwein, J.A. Wolny, Chem. Phys. Lett. 429 (2006)189.
 D. Chernyshov, M. Hostettler, K.W. Törnroos, H.-B. Bürgi, Angew. Chem., Int.Ed. 42 (2003) 3825.
 J. Kusz, D. Schollmeyer, H. Spiering, P. Gütlich, J. Appl. Crystallogr. 38 (2005)528.
 Y. Miyazaki, T. Nakamoto, S. Ikeuchi, K. Saito, A. Inaba, M. Sorai, T. Tojo, T.Atake, G.S. Matouzenko, S. Zein, S.A. Borshch, J. Phys. Chem. B 111 (2007)12508.
 S. Decurtins, P. Gütlich, C.P. Kohler, H. Spiering, A. Hauser, Chem. Phys. Lett.139 (1984) 1.
 A. Hauser, Coordin. Chem. Rev. 111 (1991) 275. A. Hauser, J. Jeftic, H. Romstedt, R. Hinek, H. Spiering, Coordin. Chem. Rev. 190–
192 (1999) 471. C.P. Slichter, H.G. Drickamer, J. Chem. Phys. 56 (1972) 2142. H. Spiering, E. Meissner, H. Köppen, E.W. Müller, P. Gütlich, Chem. Phys. 58
(1982) 65. J.F. Létard, G. Chastanet, O. Nguyen, S. Marcen, M. Marchievie, P. Guionneau, P.
Chasseau, Monatsch. Chem. 134 (2003) 165.
 F. Varret, K. Boukheddaden, E. Codjovi, C. Enachescu, J. Linares, Top. Curr.Chem. 234 (2004) 199.
 M. Sorai, Y. Maeda, H. Oshio, J. Phys. Chem. Solids 51 (1990) 941. C. Enachescu, H. Constant-Machado, N. Menendez, E. Codjovi, J. Linares, F.
Varret, A. Stancu, Physica B 306 (2001) 155. C. Enachescu, R. Tanasa, A. Stancu, G. Chastanet, J.F. Letard, J. Linarès, F. Varret,
J. Appl. Phys. 99 (2006) 08J504. N. Huby, L. Guérin, E. Collet, L. Toupet, J.-C. Ameline, H. Cailleau, T. Roisnel, T.
Tayagaki, K. Tanaka, Phys. Rev. B 69 (2004) 020101. G. Molnar, A. Bousseksou, A. Zwick, J.J. McGarvey, Chem. Phys. Lett. 367 (2003)
593. A. Goujon, B. Gillon, A. Debede, A. Cousson, A. Gukasov, J. Jeftic, G.J. McIntyre, F.
Varret, Phys. Rev. B 73 (2006) 104413. R. Tanasa, C. Enachescu, A. Stancu, E. Codjovi, J. Linares, F. Varret, J. Haasnoot,
Phys. Rev. B 71 (2005) 014431. C. Enachescu, R. Tanasa, A. Stancu, F. Varret, J. Linarès, E. Codjovi, Phys. Rev. B
72 (2005) 054413. R. Tanasa, C. Enachescu, A. Stancu, F. Varret, J. Linares, E. Codjovi, Polyhedron
26 (2007) 1820. R. Bronisz, Inorg. Chem. 44 (2005) 4463. I. Krivokapic, C. Enachescu, R. Bronisz, A. Hauser, Chem. Phys. Lett. 455 (2008)
192. A. Hauser, P. Gütlich, H. Spiering, Inorg. Chem. 25 (1986) 4245. C. Enachescu, U. Oetliker, A. Hauser, J. Phys. Chem. B 37 (2002) 9540. K. Boukheddaden, J. Linares, H. Spiering, F. Varret, Eur. Phys. J. B 15 (2000) 317. F. Varret, K. Boukheddaden, C. Chong, A. Goujon, B. Gillon, J. Jeftic, A. Hauser,
Europhys. Lett. 77 (2007) 30007. V. Niel, A.L. Thompson, A.E. Goeta, C. Enachescu, A. Hauser, A. Galet, M.C.
Munoz, J.A. Real, Chem. Eur. J. 11 (2005) 2047. E. Freysz, S. Montant, S. Létard, J.F. Létard, Chem. Phys. Lett. 394 (2004) 318.